GaN/Gd2O3/GaN Single Crystal Heterostructure …GaN on Gd2O3. Fig. 2 XTEM showing the structure of...
Embed Size (px)
Transcript of GaN/Gd2O3/GaN Single Crystal Heterostructure …GaN on Gd2O3. Fig. 2 XTEM showing the structure of...
GaN/Gd2O3/GaN Single Crystal Heterostructure (Invited)
M. Hong, J. Kwo, S. N. G. Chu, and J. P. Mannaerts Agere Systems, Inc., Murray Hill, New Jersey, USA
A. R. Kortan, H. M. Ng, A. Y. Cho, and K. A. Anselm#
Bell Labs, Lucent Technologies, Murray Hill, NJ # Now at Applied Optoelectronics Inc., Sugar Land, Texas
C. M. Lee, and J. I. Chyi EE Dept., National Central U., Taiwan, ROC
It is fascinating to study the epitaxy of two dissimilar materials and to explore new applications and novel physical phenomena built on such heterostructures. The attainment of single crystal oxides epitaxially grown on semiconductors has been previously reported. Although it is more difficult to achieve good epitaxial growth of semiconductors on oxides, a notable example was found in the growth of single crystal GaN on sapphire. Rare earth oxides are among a group of oxides, which earlier were found to grow epitaxially on GaAs and Si. These oxides recently have attracted a lot of attention because of applications on passivating semiconductor surfaces. In the area of III-V compound semiconductors, deposition of Gd2O3 films on clean GaAs surfaces in UHV has produced a low interfacial density of states (Dit). This is essential in making metal oxide semiconductor field effect transistors (MOSFET’s) with inversion in GaAs and its related compounds. Y2O3, Gd2O3, and Pr oxides on Si give low electrical leakage currents, a low Dit, and high dielectric constants, important aspects for replacing SiO2 as gate dielectrics for Si-based transistors.
In this work, not only single crystal rare earth oxide films (Gd2O3) were grown epitaxially on single crystal GaN films, but also single crystal GaN films were shown to overgrow epitaxially on the rare earth oxide films. The GaN films grown on sapphire (Al2O3) (0001) have a wurtzite hexagonal close-packed (hcp) structure. RHEED patterns of the UHV-annealed GaN show six-fold symmetry (Fig. 1 (a)), in which the pattern on the left was taken along the azimuthal and the one on the right along the direction, with a 30° separation. During the initial growth of Gd2O3 on GaN, streaky RHEED patterns with a six-fold symmetry were observed. The two major in-plane directions of the oxide (Fig. 1 (b)) are aligned with those of GaN. This is very different from the two- and four-fold symmetry pattern observed in the growth of Gd2O3 on GaAs. The same heterostructure has also been obtained with another rare earth oxide of Y2O3 replacing Gd2O3. The Gd2O3 films grown on the GaN were, unexpectedly, found to have an hcp structure. The GaN epilayers overgrown by MBE on the rare earth oxide films have a wurtzite hcp structure. Fig. 1 (a) RHEED patterns of GaN surface and (b) RHEED of Gd2O3 film 18 Å thick deposited on GaN.
The XTEM micrographs (Fig.2) were taken using a  reflection, a condition used to reveal the screw and mixed dislocations in GaN layers. The bottom GaN layer shows a typical threading dislocation structure in a MBE grown GaN layer on sapphire substrate. However, growth of a thin Gd2O3 layer on such GaN layer is expected to terminate the threading dislocations due to a different crystal structure of Gd2O3. The distinct contrasts of the screw and mixed dislocations all terminate at the bottom interface of a thin Gd2O3 layer. Since the growth of the top GaN layer has to be re-initiated on the Gd2O3 surface, a different dislocation structure is expected to form. The wavy and tangle nature of the dislocation structure in the top GaN layer as seen in
Fig. 2 does indicate a different nucleation process for GaN on Gd2O3.
Fig. 2 XTEM showing the structure of GaN/Gd2O3/GaN. It was unexpected that an hcp Gd2O3 single
crystal would grow on GaN, considering that the hcp structure exists only at temperatures over 2000
was also surprised that the GaN single crystal would grow on the hcp rare earth oxides. In an ellipsometry study of hcp Gd2O3, a refractive index of 2.0-1.94 was measured in the wavelength range of 400-800 nm. The large refractive index difference between the rare earth oxide and GaN may find applications in photonic devices. We have also obtained a low Dit of ~1011 cm-2eV-1 for the rare earth oxide/GaN interface. The attainment of a low interfacial density of states in the rare earth oxide single crystal thin films UHV-deposited on GaN may find applications in opto-electronic and electronic devices such as MOSFETs.